LIQUID PHASE REARRANGEMENT OF LONG STRAIGHT-CHAIN EPOXIDES
OVER AMORPHOUS, MESOSTRUCTURED AND ZEOLITIC CATALYSTS
David P. Serrano, Rafael van Grieken, Juan Antonio Melero* and Alicia García
Chemical and Environmental Engineering Group, ESCET, Rey Juan Carlos University,
c/ Tulipán s/n, 28933, Móstoles, Spain.
Applied Catalysis A: General, 269 (2004) 137-146
Tel: +34 91 488 70 87. Fax: +34 91 488 70 68
A variety of materials with different structural features and acid properties, including
amorphous, mesostructured and zeolitic catalysts have been tested in the liquid-phase
rearrangement of 1,2-epoxyoctane. The structure and acid strength of the catalysts influence
strongly on the activity and product selectivity. The main rearrangement products are the
aldehyde, allylic alcohols and diol. Acid sites in the amorphous materials show a poor catalytic
activity. Al-TS-1 and Al-Ti-beta, zeolites with medium aluminium content, lead to significant
activities and selectivities towards both the aldehyde and the octenols in comparison to those
obtained with other zeolitic materials tested. Aluminium-containing mesostructured materials
present much higher activities than amorphous and zeolitic catalysts. Al-MCM-41 synthesized
by a sol-gel method at room temperature yielded selectivities to octaldehyde and octen-1ols of
40.6% and 44.7%, respectively with a high catalyst activity (TOF of ca. 30.5).
Hydroformilation of terminal alkenes, from his discovery by Roelen in 1938, has been
used conventionally as one of the most versatile methods for the functionalization of terminal
alkenes into carbonyl compounds. This process is based on the addition of carbon monoxide and
hydrogen to the alkene double bond to yield aldehydes that can be subsequently hydrogenated
to terminal alcohols or oxidized towards the corresponding carboxylic acids [1, 2]. However,
this process has important drawbacks such as the high pressure, the use of high-cost
homogeneous catalysts or the purification of the products. Moreover, the recovery of the
rhodium-based catalysts is not an easy task. Other possible way for the synthesis of oxygenates
from terminal olefinic compounds is the oxidative cleavage of the double bond to produce
carbonyl groups. Several methods are available for this target, including the use of
stoichiometric reagents such as potassium permanganate and ruthenium tetraoxide, and complex
catalytic systems with ozone and hydrogen peroxide [3, 4]. Nevertheless, this alternative
involves a loss of the terminal carbon atom that makes inefficient the process from the point of
view of atom economy.
Since both methods above mentioned for the preparation of carbonyl compounds show
significant drawbacks, the development of an alternative process is an interesting goal. In this
way, catalytic rearrangement of epoxides towards aldehydes has been shown as an attractive
strategy of synthesis in Fine Chemistry. A number of studies on the catalytic rearrangement of
epoxides have been reported, although most of them have dealt with homogeneous acid or base
catalysts (e.g. BF3, MgBr2, ZnCl2, t-BuOK or lithium dialkylamides), whereas most of the substrates tested were highly reactive epoxides (cyclic-alkane, alkyl-aromatic and tertiary
epoxides) [5, 6]. Acid-catalyzed epoxide rearrangement leads, usually to, ketones and
aldehydes, whereas the base-catalyzed reaction of such derivatives yields allylic alcohols as
The use of homogeneous catalysis presents numerous drawbacks: loss of the catalyst
after reaction, corrosivity, toxicity and in most cases generation of contaminated streams.
Accordingly, many efforts have been addressed to find out heterogeneous catalysts to overcome
these problems. For this reason heterogeneous catalysts such as SiO2, Al2O3, ZrO2, TiO2 or physical mixtures of them have been tested for epoxide rearrangement reactions . The use of
these conventional catalysts often results in the formation of aldol condensation products and
mixtures of ketones and aldehydes as by-products. The voluminous molecules formed by aldol
condensation are the first step in the formation of coke thus limiting the lifetime of these
catalysts. Consequently, in the last years, zeolitic materials have attracted the attention because
of their well defined pore system that may suppress the side reactions mentioned above [8-11].
A number of zeolites, including HZSM-5, H-Beta, Mordenite, Zeolite Y and X, have
been tested in the rearrangement of aromatic or cyclic alkane epoxides as well as of epoxides
with tertiary carbons linked to the oxirane ring. Thus, high selectivities to aldehydes have been
obtained in the isomerization of styrene oxide and derivatives over various acid zeolites [12,
13]. Likewise, some works have been published on the use of zeolites as catalysts in the
isomerization of small size aliphatic epoxides, such as propylene oxide and
2-methyl-2,3-epoxybutene, but in addition to the desired aldehyde different by-products were obtained [14,
15]. However, few results have been reported in regards to the rearrangement of long
straight-chain 1,2-alkane epoxides. It must be pointed out that these kind of epoxides are low reactive
substrates, hence the isomerization to the corresponding aldehyde involves stronger reaction
conditions (higher temperature, catalyst loading and reaction time) and more active catalysts
[16, 17]. An important amount of different monounsaturated terminal alcohols is also obtained
using this kind of epoxides as substrate.
Linear aldehydes can be easily oxidised towards the corresponding carboxylic acid.
mainly based on their synthetic utility. Much of them are used as intermediates for textile
chemicals, dyes, drugs, plastics and agricultural chemicals. Both linear aldehydes and
monounsaturated terminal alcohols can be also selectively hydrogenated to the corresponding
linear alcohols. Industrially, the higher alcohols can be separated into plasticizers (C6-C11) and fatty alcohols (C12-C18), used for detergents. Moreover, aliphatic alcohols are used as solvents and diluents for paints, as intermediates in the manufacture of esters and in the preparation of a
wide range of organic compounds.
These previous works prompted us to study the catalytic rearrangement of long
straight-chain epoxides in liquid phase over different acid solid catalysts. The present paper describes
the results obtained in the rearrangement of 1,2-epoxyoctane, chosen as a model epoxide, over
different acid catalysts. We have checked the activity of several catalysts having a variety of
acid properties and structural features, including different zeolites, amorphous and
2.1. Catalysts preparation
2.1.1. Amorphous materials
An amorphous SiO2-TiO2 xerogel was prepared through a two-step sol-gel method involving acid-hydrolysis of the precursors and basic gelation . Alumina and alumina-silica
2.1.2. Zeolitic materials
TS-1 zeolite was synthesized by hydrothermal crystallization of wetness impregnated
SiO2-TiO2 amorphous xerogels . ZSM-5 zeolite was prepared by a conventional method from ethanol-containing gels . Al-TS-1 and Al-Ti-beta zeolites were prepared by
hydrothermal crystallization of wetness impregnated SiO2-TiO2-Al2O3 xerogels [20, 21]. Al-beta zeolite, free of titanium, was prepared by hydrothermal synthesis in fluoride medium .
Two additional zinc-containing zeolites, CIT-6 and VPI-8 with BEA and VPI framework
topology, respectively, were synthesized under hydrothermal treatment of clear hydrogels
containing tetraethylammonium (TEA+), Li+ and Zn2+ cations . Ultra-stable Y zeolite (USY) and mordenite were supplied by Grace and Zeolyst, respectively.
2.1.3. Mesostructured materials
Al-MCM-41 (SG) was synthesized by a sol-gel procedure at room temperature using
aluminium isopropoxide as aluminium source . Additionally, a different Al-MCM-41
material, denoted as Al-MCM-41 (HT), was synthesized by a conventional hydrothermal
treatment in basic medium . Al-SBA-15 was prepared by a sol-gel procedure using Pluronic
123 triblock copolymer (EO20-PO70-EO20; Aldrich) as polymeric template and aluminium isopropoxide as aluminium source .
2.2. Catalysts Characterization
All the catalytic samples were characterized by different techniques. Crystallinity of
zeolitic samples and mesoscopic ordering of mesostructured materials were checked through
X-Ray diffraction (XRD) patterns acquired with a Philips X´PERT MPD diffractometer using Cu
0.6 to 4º (2θ) for mesostructured materials with a resolution of 0.02º. Chemical analyses of the
samples were performed by induced coupled plasma-atomic emission spectroscopy (ICP-AES)
with a Varian VISTA-AX apparatus.
Nitrogen adsorption-desorption isotherms at 77 K of the calcined catalysts were
obtained using a Micromeritics ASAP 2010 porosimeter. Previously, the samples were
outgassed under vacuum at 200 ºC for 5h. The surface areas were determined according to the
BET equation. Pore size distribution was obtained applying the BJH method to the adsorption
branch of the isotherm. Cylindrical pore geometry was assumed for the calculations and the
Jura-Harkins equation was used to determine the thickness of the adsorbed layer. The total pore
volume was determined from the N2 adsorption at p/p0=0.99. Micropore volume and external surface area of the catalysts were determined using the t-plot method. Morphology and size of
the catalyst particles were obtained by scanning electron microscopy (SEM) with a JEOL JSM
The coordination of the aluminum atoms in the catalysts was checked by 27 Al-MAS-NMR spectra of the calcined samples. The spectra were recorded at 104.26 MHz in a VARIAN
Infinity 400 spectrometer at spinning frequency of 4 KHz and intervals ranging from 5 to 30 s
between successive accumulations were selected according to the structural nature of the
sample. The external standard reference was [Al(H2O)6 +3
] and all measurements were carried
out at room temperature.
The acid properties of the catalysts were determined by ammonia temperature
programmed desorption (TPD) in a Micromeritics 2910 (TPD/TPR) equipment. Previously, the
samples were outgassed under an helium flow (50 Nml min-1) with a heating rate of 15 ºC min-1 up to 560 ºC and kept at this temperature for 30 min. After cooling to 180 ºC, an ammonia flow
removed by flowing helium at 180 ºC for 90 min. The chemically adsorbed ammonia was
determined by increasing the temperature up to 550 ºC with a heating rate of 15 ºC min-1, this temperature being kept for 30 min. The ammonia concentration in the effluent helium stream
was measured through a thermal conductivity detector (TCD).
2.3. Catalytic experiments
The catalytic experiments were carried out in a 0.1 L stirred batch autoclave equipped
with a temperature controller and a pressure gauge at 120ºC for different reaction times under
stirring (550 rpm) and autogenous pressure. This experimental set-up is also provided with a
device to feed the epoxide into the teflon-lined reactor once the reaction temperature is reached.
The solvent and the catalyst are initially placed in the teflon-lined reactor. The zero time of the
reaction is considered when the temperature reaches the set-point value and the epoxide is
loaded into the reactor. The composition of the reaction mixture was as follows: 1 g of
1,2-epoxyoctane, 20 g of toluene (water content less than 0.03 wt. %) and 40 or 200 mg of catalyst
depending on its activity. Toluene was stored with A zeolite to minimize its water content. The
catalyst, prior reaction, was dried overnight at 140 ºC.
The reaction products were analyzed with a GC (VARIAN 3800) equipped with a
capillary column (HP-FFAP) with dimensions 60 x 0.32 mm, using a flame ionization detector
(FID). Identification of the different reaction products was also performed by mass spectrometry
3. Results and discussion
3.1 Catalysts properties
The main physicochemical and textural properties of the catalysts used in this work are
summarized in Tables 1, 2 and 3 for the amorphous, zeolitic and mesostructured materials,
respectively. The SiO2-TiO2 xerogel synthesised through a two-step sol-gel method  is an amorphous material with high surface area characterised for possessing weak Lewis acid sites,
not detected in the NH3 TPD measurements. It shows a mesopore size distribution centered at 50 Å. Al2O3 and SiO2-Al2O3 samples are amorphous solid oxides with stronger Lewis acidity, although lower surface area compared to the SiO2-TiO2 xerogel.
Table 1. Physicochemical properties of the amorphous catalysts.
Catalyst Molar Ratio
Surface Area (m2 g-1)
Pore Volume (cm3 g-1)a
Acidity (mmol g-1)b
T max (ºC)b
SiO2-TiO2 Si/Ti: 52 50 550 0.60 0.00 -
Al2O3 - 48 133 0.25 0.45 260
SiO2-Al2O3 Si/Al: 15 22-120 261 0.97 0.19 284
a Measured at P/P
0 = 0.99. b
Acid capacity and maximum desorption temperature in TPD measurements
Considering their pore diameters the microporous materials tested can be classified in
medium and large pore size zeolites (Table 2). TS-1, ZSM-5 and Al-TS-1 are medium pore size
zeolites with a pore diameter around 5.5 Å and a three-dimensional pore structure (MFI
topology). Al-Ti-Beta and Al-Beta zeolites are large pore size zeolites with a three-dimensional
BEA structure which possesses tortuous 12-membered ring channels along c-direction, having a
cross section of 5.6 x 6.5 Å. These channels intersect with a set of straight 12-membered ring
ultra-stable Y zeolite (USY) are microporous materials with a large pore size characterized by
possessing a higher aluminium content compared to the other zeolitic materials. Mordenite
presents a one-dimensional pore system with a pore diameter of 6.5 x 7.0 Å, whereas USY
zeolite possesses a three-dimensional large pore system (7.4 Å) with supercages of 12 Å. CIT-6
and VPI-8 are both large pore crystalline zincosilicates, but with a different framework
topology. CIT-6 presents BEA structure whereas VPI-8 is characterized by a one-dimensional
pore system with a pore diameter of 5.9 Å. These two materials have been selected as catalyst in
this work due to high activities and selectivities obtained in epoxide rearrangement processes
with zinc chloride as homogeneous catalyst.
Table 2. Physicochemical properties of the zeolitic catalysts
Catalyst Molar Ratio Pore Diameter (Å) Dc (µm)a Surface Area (m2 g-1)
Micropore Volume (cm3 g-1)b
Acidity (mmol g-1)c
T max (ºC)c
Medium pore size TS-1 Si/Ti: 40 5.4 x 5.4
5.1 x 5.7
0.5-0.7 525 0.18 0.00 -
ZSM-5 Si/Al: 30 5.4 x 5.4 5.1 x 5.7
5.0-7.0 495 0.17 0.43 358
Al-TS-1 Si/Al: 122 Si/Ti: 83
5.4 x 5.4 5.1 x 5.7
0.3-0.4 490 0.19 0.17 331
Large pore size Al-Ti-Beta Si/Al: 41
5.6 x 6.5 5.7 x 7.5
0.2-0.3 552 0.23 0.47 319
Al-Beta Si/Al: 57 5.6 x 6.5 5.7 x 7.5
1.0-1.2 567 0.26 0.20 285
Mordenite Si/Al: 11 6.5 x 7.0 0.1-0.5 535 0.23 0.56 408
USY Si/Al: 3.5 7.4 0.7-1.0 436 0.19 0.37 277
Zn-containing zeolites CIT-6 Si/Zn: 16 5.6 x 6.5
5.7 x 7.5
0.8-1.1 495 0.22 0.11 247
VPI-8 Si/Zn: 24 5.9 x 5.9 1.0-1.4 450 0.19 0.03 231
Mean crystal size.
b Measured at P/P
0 = 0.99.
From the NH3 TPD results shown in Table 2, it can be seen that the acid strength in zeolites depend not only on the aluminium content but also on the catalysts topology. Mordenite
present the highest strength of acid sites with a peak maxima of ammonia desorption placed at
408 ºC. ZSM-5, Al-TS-1 and Al-Ti-beta exhibit sites of intermediate acid strength (Tmax = 358, 331 and 319 ºC, respectively) compared to those of mordenite zeolite and the rest of catalysts.
The aluminium-containing zeolitic materials were analyzed by 27Al-MAS NMR in order to bear out the degree of aluminium incorporated into the zeolitic framework. All the samples show a
distinct peak at 52 ppm corresponding to tetrahedral aluminium and a fairly small one placed at
~0 ppm assigned to the presence of low amounts of extraframework aluminium species with
octahedral coordination. Zn-containing zeolites show acid sites with the lowest strength as
concluded by the maximum desorption temperature in NH3 TPD experiments of ca. 240 ºC.
Al-MCM-41 (SG) and Al-MCM-41 (HT) are ordered mesoporous materials synthesized
by two different methods, a sol-gel method at room temperature and a hydrothermal method in
basic conditions, respectively. Although both samples have similar chemical composition with
pore sizes above 2.0 nm, some significant differences are observed in their acid and textural
Table 3. Physicochemical properties of the mesostructured catalysts.
Catalyst Molar Ratio
Surface Area (m2 g-1)
Pore Volume (cm3 g-1)a
Acidity (mmol g-1)b
T max (ºC)b
Al-SBA-15 Si/Al: 76 50 550 0.49 0.19 284
Al-MCM-41 (SG) Si/Al: 39 21 1087 0.68 0.28 275
Al-MCM-41 (HT) Si/Al: 36 23.5 1015 0.62 0.18 266
a Measured at p/p
0 = 0.99.
Figure 1 shows the nitrogen adsorption-desorption isotherms at 77 K and pore size
distributions corresponding to Al-MCM-41 (SG) and Al-MCM-41 (HT) samples. The two
isotherms in Figure 1.a are clearly of type IV, which are typical of mesoporous materials. The
inflections points observed at relative pressures around 0.2 indicate that capillary condensation
in mesopores occurs after the monolayer adsorption on the walls. For relative pressures above
0.5, the isotherms present an almost constant adsorption zone that, in the case of Al-MCM-41
(SG), suffers a significant increase at high relative pressures due to multilayer formation on the
external surface of the particles. Significant differences can be appreciated in the pore size
distributions of Figure 1.b. The Al-MCM-41 (SG) sample presents a wider pore size distribution
and smaller pores with sizes in the micro-mesopore limit as compared to that observed for
Al MAS NMR spectra of both Al-MCM-41 samples after calcination show two clear
peaks centred at ~4 ppm and ~50 ppm originated from octahedrally and tetrahedrally
coordinated aluminium species, respectively. The relative proportion of octahedral to tetrahedral
species is higher in Al-MCM-41 (HT) than in Al-MCM-41 (SG) and in both cases larger than
that observed in zeolites. Al-SBA-15 is also a hexagonally ordered mesostructured material but
with textural properties significantly different from Al-MCM-41. It exhibits a higher pore size,
around 50 Å, a BET surface area appreciably lower, arising from a higher wall thickness, and
the presence of complementary micropores located on the silica wall and providing connectivity
between the mesostructured channels . All the mesostructured materials possess acid sites
with medium acid strength since their temperature maxima for ammonia desorption are placed
0,0 0,2 0,4 0,6 0,8 1,0 0 100 200 300 400 500 600 a) A d so rb e d v o lum e ( S T P cm 3 /g ) P/P O 10 100 0,00 0,01 0,02 0,03 0,04 0,05 0,06 b) d V / d log D ( cm
Pore Diameter (A)
Figure 1. N2 adsorption-desorption on the Al-MCM-41 materials: a) isotherms, b) pore size distributions
( ) Al-MCM-41 (SG) ( ) Al-MCM-41 (HT).
3.2. Catalytic epoxide rearrangement
The results obtained over the different catalytic systems in the isomerization of
1,2-epoxyoctane in liquid phase are shown in Tables 5, 6 and 7 in terms of activity and product
frequency (TOF) defined, as moles of reacted epoxide per mol of active site and hour. Since
some epoxides may be isomerized thermally, a blank reaction in absence of catalyst was carried
out that yielded a negligible conversion under the reaction conditions used in this work.
Most of the catalysts tested promote the isomerization of the epoxide towards the
corresponding aldehyde (1) and ketone (2) through carbocation-mediated processes and
subsequent 1,2-shift (Scheme 1). Additionally, other two important secondary reactions are also
detected: the formation of different octenols coming from positive charge shift of one of the
carbocations generated (Scheme 2) and diol generation by nucleophilic attack of water to the
oxirane ring (Scheme 3). The formation of the different octenols (3 and 4) and of
1,4-epoxyoctane (5) is explained in terms of the different transpositions of the positive charge of the
carbocation (Scheme 2). In all cases, the main product coming from these secondary reactions is
2-octen-1-ol (3) since the formation of allylic alcohols is always favoured. The appearance in
the reaction product of relatively large amounts of diol indicates the presence of water probably
contained in the solvent and/or originated from the dehydroxilation of silanols groups located on
the surface of the catalysts.
R CH2 CH CH2 O R CH2 CH CH2
O H +
R CH2 CH CH2 OH +
R CH2 CH2 C O H
R CH2 C CH3 O H +
+ R CH2 CH CH2
CH3 (CH2)3CH2-CH2-CH CH2 OH +
CH3(CH2)3CH2-CH CH-CH2 OH
CH3(CH2)3CH CH-CH2-CH2 OH
CH3(CH2)3CH2-CH-CH2 CH2 OH
CH3(CH2)3CH-CH2-CH2 CH2 OH + + H+ + H + H
Scheme 2. Transposition of the positive charge in 1,2-epoxyoctane leading to different octenols and 1,4-epoxyoctane: (3) 2-octen-1-ol, (4) 3-octen-1-ol and (5) 1,4-epoxyoctane.
H H +
R CH2 CH CH2
R CH2 CH CH2
R CH2 CH CH2
Scheme 3. Nucleophilic attack by water of the oxirane ring in 1,2-epoxyoctane: (6) 1,2-octanediol.
Another type of product obtained in the rearrangement reaction of 1,2-epoxyoctane over
heterogeneous catalysts is 2-oct-2-enyloxy-octan-1-ol, (7), whose presence has been confirmed
by mass spectrometry indicating a C16 structure (m/e=256). We postulate that this compound is formed by the nucleophilic attack of octenols to the epoxide as outlined in Scheme 4. With the
purpose of confirming the formation mechanism of this compound we have performed an
enhancement of the formation of compound (7) in comparison with the reaction carried out in
absence of the allylic alcohol.
Scheme 4. Nucleophilic attack of octenols to the epoxide: (7) 2-oct-2-enyloxy-octan-1-ol.
Some authors have postulated the formation of significant amounts of condensation
products coming from a consecutive reaction of the aldehyde itself . With the purpose of
clarifying the possible formation of these kind of products under the reaction conditions
described in this work, an additional catalytic run of aldolic condensation of octaldehyde over
mordenite at 120 ºC for 3 hours using toluene as solvent was carried out. A unique reaction
product was obtained but with a retention time in chromatograph analysis different to that of
compound numbered as (7). Likewise, this condensation compound is not detected in the
isomerization reactions performed in this work (Tables 5, 6 and 7). These catalytic experiments
clearly confirm that compound (7) is coming from nucleophilic attack of allylic alcohol to the
Table 4. 1,2-Epoxyoctane rearrangement over ZnCl2 in presence and absence of 2-octen-1-ol
Run Conversion(%) Product distribution (mg)
1 3 4 6 2+5 7
1a 98.3 379 111 0 45 122 240
2b 98.7 461 1068 45 2 20 530
a Reaction conditions: 1,2-epoxyoctane: ca. 1 g; ZnCl
2: 200 mg; time: 3 h. b
Reaction conditions: 1,2-epoxyoctane: ca. 1 g ; 2-octen-1-ol: ca. 1 g; ZnCl2: 200 mg; time: 3 h.
The screening of the different catalytic systems has been carried out on the basis of their
catalytic activity and selectivity towards valuable products such as aldehydes and octenols.
Linear aldehydes can be conveniently transformed into linear carboxylic acids or terminal
alcohols, important precursors in Organic Chemistry. Moreover, octenols can be also selectively
hydrogenated to linear alcohols .
3.2.1. Epoxide rearrangement over amorphous catalyts.
Three different amorphous oxides (SiO2-TiO2 xerogel, Al2O3 and SiO2-Al2O3) have been tested in the liquid phase rearrangement of 1,2-epoxyoctane, obtaining the results shown in
Table 5. The SiO2-TiO2 xerogel evidences a very low activity, which correlates fairly well with its low acid strength shown by the ammonia TPD results. The activity obtained over Al2O3 was not higher than that of the blank reaction whereas the SiO2-Al2O3 catalyst presents a conversion somewhat higher than that obtained with the SiO2-TiO2 xerogel. In terms of TOF both mixed oxides behave in a similar way, but the product distribution obtained is quite different. The
SiO2-TiO2 xerogel leads to a significant formation of diol (ca. 40.6%), probably related with the high content of hydroxyl groups present in this material, with low octaldehyde selectivity.
valuable products (octaldehyde+octen-1-ols: 55.6%). These catalytic results demonstrate that
these materials do not catalyze effectively the isomerization of linear epoxides.
Table 5. 1,2-Epoxyoctane rearrangement over amorphous catalystsa Catalyst Conversion
TOFb Selectivity (%)
1 3+4 6 2+5 7 SiO2-TiO2 4.3 1.8c 12.3 37.2 40.6 5.4 4.5
Al2O3 0.0 0.0 - - - - -
SiO2-Al2O3 14.3 1.9 33.4 22.2 22.9 3.7 17.8 a
Reaction conditions: catalyst loading: 200 mg; time: 3 h.
b mol 1,2-epoxide converted/(mol Al·h) after 3 hours c Activity per mol of Ti.
3.2.2. Epoxide rearrangement over zeolitic catalysts.
A number of works have been published regarding the use of zeolites as catalysts in
epoxides isomerizations. The interest in such solids as catalysts in these kind of processes arises
from their well defined pore system and high stability. Hölderich et al. have disclosed the
rearrangement of 2-methyl-2,3-epoxybutene, 2-methylstyrene oxide and diisobutylene oxide to
yield aldehydes in the presence of various zeolites of the pentasil type [29, 30]. Propanal can be
prepared in gas phase from propylene oxide rearrangement over basic zeolites such as (Mg,
Na)-Y with selectivities up to 88% . Brunel et al.  have reported the 1,2-epoxyoctane
rearrangement over zeolites HY, H-OFF and H-beta with selectivities towards octanal and
allylic alcohol around 45% and 25%, respectively.
Taking these previous results as reference, we decided to test a variety of zeolitic
materials with different framework topology and acid strength in the liquid phase rearrangement
of 1,2-epoxyoctane. The results obtained have been summarized in Table 6. At the first attempt,
of strong Brönsted acid sites, was firstly tested. The activity results (TOF ca. 2.3) clearly
indicate that the weak acid Lewis sites present in TS-1 does not promote properly the epoxide
rearrangement. When a sample of ZSM-5 (Si/Al molar ratio of 30) was used as catalyst an
increase in both TOF and conversion was observed, but no significant changes regarding the
product distribution were detected.
Al-TS-1 with bifunctional properties due to the simultaneous presence of titanium and
aluminium in the zeolite framework has been also tested. The results obtained suggest that acid
sites in Al-TS-1 show a similar activity to those present in ZSM-5 sample. The higher
conversion observed over ZSM-5 might be attributed to its higher aluminium content, although
a greater value should be expected. This could be explained considering internal diffusional
problems arising from the larger crystal size of ZSM-5 sample (5-7 µm) compared to that of
Al-TS-1 (0.3-0.4 µm). From the results shown in Table 6, it can be observed that Al-Al-TS-1 yields a
higher amount of valuable products (octaldehyde+octen-1-ols: 74.5%) in comparison to the
selectivities obtained with TS-1 and ZSM-5 zeolites.
Al-containing zeolites with larger pore size have been also investigated in order to promote
the access of the substrate within the catalyst pores and avoid diffusional limitations. Al-Ti-Beta
zeolite shows a similar activity per mol of acid site than Al-TS-1 and ZSM-5 but a higher
epoxide conversion, probably due to its larger pore size. In contrast with the product distribution
obtained with Al-TS-1, Al-Ti-Beta leads to an enhancementin the formation of 1,2-octanediol
what decreases the selectivity towards valuable products (ca. 66.3%). Besides, another catalytic
run has been carried out in presence of Al-beta zeolite synthesised by hydrothermal
crystallization in a neutral medium (fluoride method). This material is characterised by
possessing a high hydrophobic surface as a consequence of the low content of structural defects
(silanols groups) in contrast with Beta zeolite samples synthesized under basic hydrothermal
hydrophobic character of the sample hinder the accessibility of the polar substrate within the
zeolite pores. Moreover, larger crystal size of the Al-beta sample compared to Al-Ti-beta could
involve some diffusional problems that are avoided in the latter due to its smaller crystallites.
Nevertheless, it is remarkable the high octen-1-ols selectivity obtained with this material (ca.
Table 6. 1,2-Epoxyoctane rearrangement over zeolitic and homogeneous catalystsa
Catalyst Conversion (%)
TOFb Selectivity (%)
1 3+4 6 2+5 7 Medium pore size zeolites
TS-1 6.4 2.3c 34.9 26.4 25.6 7.0 6.1
ZSM-5 24.5 6.2 33.6 31.2 20.8 9.2 5.2
Al-TS-1 13.5 5.0d 25.3 49.2 15.1 7.7 2.7
Large pore size zeolites
Al-Ti-Beta 36.2 6.4d 29.3 37.0 23.8 6.7 3.2
Al-Beta 5.9 2.4 12.0 65.3 16.3 0.0 6.4
Mordenite 41.4 3.7 35.6 32.7 20.7 5.0 6.0
USY 10.3 0.4 18.2 46.7 29.2 4.3 1.6
CIT-6 10.7 1.3e 3.9 77.6 17.1 0.0 1.4
VPI-8 0.0 0.0e 0.0 0.0 0.0 0.0 0.0
ZnCl2 46 2.4e 59.8 5.9 0.9 5.8 27.6
Reaction conditions: catalyst loading: 200 mg; time: 3 h.
b mol 1,2-epoxide converted/(mol Al·h) after 3 hours c Activity per mol of Ti;
d Activity per mol of Al+Ti e
Activity per mol of Zn.
In order to gain more information about the catalytic performance of different zeolitic
materials in this particular reaction, materials with a high aluminium content such as mordenite
(Si/Al: 11; Dp: 6.5 x 7.0 Å) and ultra-stable Y zeolite (Si/Al: 3.5; Dp: 7.4 Å) have been also
investigated. Under the conditions depicted in Table 6, mordenite sample shows the highest
epoxide conversion with a value of around 41%. However, the activity per mol of active site
obtained is low (TOF: 3.7) probably due to the one-dimensional pore system of this zeolite
which could hinder the accessibility of reactants to the active sites. Ultra-stable Y zeolite, with a
three-dimensional large pore system (7.4 Å), led to a low epoxide conversion and an almost
negligible activity (10.3 % and 0.4, respectively). These results are quite different from those
reported by Hölderich et al. in the rearrangement of α-pinene oxide over USY zeolite .
However our catalytic results illustrate clearly the lower reactivity of long-straight chain
epoxides. The product distribution obtained when mordenite is used as catalyst is similar to the
results shown by ZSM-5 sample, whereas USY zeolite leads to the highest diol selectivity (ca
29.3%) and a high amount of octen-1-ols (ca. 46.7%).
Finally, since zinc chlorides are known to be effective homogeneous catalysts in
epoxides rearrangement , we have considered the use of zinc-containing zeolites in this kind
of process. Thus, two zinc-containing zeolites with BEA and VPI structure, characterised for
possessing Lewis acid sites were used as catalysts and compared with ZnCl2. The catalytic results obtained over VPI-8 zincosilicate were disappointing, since it showed a negligible
activity. In contrast, the CIT-6 zincosilicate presented an epoxide conversion similar to that of
Al-TS-1 zeolite but with a lower activity per mol of active site. The product distribution
obtained over CIT-6 is interesting due to the high octen-1-ols selectivity obtained (ca. 77.6%). It
is noteworthy that the use of the homogeneous catalytic system, ZnCl2, leads to a low activity per mol of active site (TOF: ca. 2.4). Likewise, this system yielded an octaldehyde selectivity of
Al-containing zeolites, but with lower octen-1-ols selectivity. Note that the formation of the bulky
(7) compound is clearly enhanced as a consequence of the absence of sterical restrictions.
In conclusion, Al-containing zeolitic materials with a medium aluminium content seems
to be active in the rearrangement of 1,2-epoxyoctane in liquid phase towards the corresponding
aldehyde and octenols although a high amount of undesirable diol is formed. Nevertheless, the
extension of the reaction seems to be dramatically influenced by the limitations of the pore and
crystal size. Note that all the zeolitic materials catalyses the formation of the bulky
2-oct-2-enyloxy-octan-1-ol compound (scheme 4) in spite of their limited pore size although in less
extent that in SiO2-Al2O3 catalyst and homogeneous system. Probably, the external acid sites of
these zeolitic materials are acidic enough to catalyse the formation of this compound.
3.2.3. Epoxide rearrangement over Al-containing mesostructured catalysts.
The discovery of mesoporous molecular sieves of the M41S family  opened new
possibilities for the preparation of catalysts with uniform pores in the mesoporous range, easily
accessible for bulky molecules and, thus, without limitations typical of microporous materials.
The possibility of incorporating aluminium into the silica walls turned these materials into
solids with acid sites of medium strength, with potential applications as acid catalysts in
different reactions (cracking, hydrocracking, etc.) . The presence of both Brönsted and
Lewis acid sites on aluminium-containing mesostructured materials prompted us to check this
kind of materials in the liquid phase isomerization of 1,2-epoxyoctane, with the purpose of
studying the influence of catalytic systems with pore sizes and acidity very different from those
present in zeolitic materials. Moreover, up the best of our knowledge, the work here reported is
the first using aluminium-containing mesostructured materials as catalysts for long-straight
Three catalytic experiments were carried using aluminium-containing SBA-15 and
MCM-41 materials synthesised in our laboratory. Preliminary experiments with these materials
(not shown) yielded a sharp enhancement of catalytic activities as compared with the catalysts
mentioned above. Therefore, a lower catalyst loading was used in order to obtain comparative
epoxide conversions (ca. 40 mg).
We found that all mesoporous materials tested present much higher activities per active
site in comparison to those obtained with zeolitic materials. These results probably arise from
the larger pores of mesostructured materials that avoid diffusional problems present in zeolitic
catalysts. Al-SBA-15 shows an activity lower than Al-MCM-41 samples in spite of the similar
strength of the acid sites obtained by TPD measurements. This fact may be assigned to the
presence of an important amount of active sites located in the microporosity of SBA-15
materials, which hinders the accessibility of the substrate.
Al-MCM-41 (SG), synthesized by a sol-gel method at room temperature, yields
selectivities to octaldehyde and octen-1-ols of 40.6% and 44.7%, respectively, which means an
overall selectivity towards valuable products near 85 %. Moreover, its catalyst activity is 10-20
times higher than those obtained with zeolites (TOF: ca. 68). Surprisingly, the catalytic results
obtained with Al-MCM-41 (HT) are very different to that showed by Al-MCM41 (SG) in terms
of product distribution. The use of Al-MCM-41 (HT) as catalyst on 1,2-epoxyoctane
rearrangement enhances the formation of a high amount of 1,2-octanediol (45.1%) with a poor
yield to valuable products (octanal+octen-1-ols selectivity: ca. 44.6%). The treatment of this
catalyst with trimethylsilane may result in an improvement of the catalytic performance towards
the formation of valuable products.
Such different results might be attributed to the different properties of the catalysts
distribution, better accessibility of acid centers (see TPD measurements in Table 3), higher
adsorption capacity of molecules and lower content of aluminium extraframework species that
may affect the catalytic behaviour. In line with our catalytic results some researchers have
postulated that less ordered mesoporous materials are generally more catalytic active than those
having ordered hexagonal pores . This enhancement of the activity may result from the
presence of interconnected mesopores that would allow easier access of substrate to the active
Table 7. 1,2-Epoxyoctane rearrangement over mesoporous materialsa
Catalyst Conversion (%)
TOFb Selectivity (%)
1 3+4 6 2+5 7
Al-SBA-15 5.9 29.2 29.6 48.2 9.4 11.4 1.4
Al-MCM-41 (SG) 30.5 67.9 40.6 44.7 7.9 5.7 1.1
Al-MCM-41 (HT) 29.0 56.6 36.1 8.5 45.1 5.0 5.3
a Reaction conditions: catalyst loading: 40 mg; time: 2 h. b
mol 1,2-epoxide converted/(mol Al·h) after 2 hours.
Finally, Figure 2 summarises the activity of the different catalytic systems in terms of
TOF as a function of the pore diameter. Amorphous SiO2-TiO2 material shows a poor catalytic
activity, which correlates with the low acid strength of their acid sites. Amorphous SiO2-Al2O3
material yields a low activity in spite of having a similar acid strength than that shown by
mesostructured materials. This fact may be attributed to the lower accessibility of acid centers
clearly evidenced in TPD measurements. In general zeolitic materials suffer from diffusional
problems, which hinder the access of the linear epoxide to the active sites. Mesostructured
Al-MCM-41 materials combine an appropriate pore size as well as a suitable accessibility and acid
strength of their active sites that allow the highest activity. In contrast, Al-SBA-15 in spite of
pore sizes yielded a low activity. This fact is probably assigned to a lower accessibility of the
active sites in this material, as they may be located in the complementary micropores existing in
the SBA-15 silica walls. Note that TOF values in mesostructured materials are about one order
of magnitude higher than in zeolites. These catalytic results show that both a medium acid
strength and high accessibility of acid sites are essential factors to obtain high activity in the
rearrangement of linear epoxides.
Figure 2. Activity of the different catalysts plotted versus the average pore size
From all the results obtained, it can be concluded that Al-MCM41 (SG) materials
present the best catalytic performance, regarding to both activity and valuable product
distribution. This kind of materials catalyzes selectively the isomerization of 1,2-epoxyoctante
leading to a mixture of the corresponding aldehyde and octen-1-ols.
0 2 4 6 8 20 40 60 80
Al-beta USY CIT-6
Al-MCM-41 (HT) Al-MCM-41 (SG)
The activity and selectivity of several catalysts with a wide range of acid properties and
structural features, including amorphous oxides, zeolites and mesostructured materials, have
been checked in the liquid phase rearrangement of 1,2-epoxyoctane. Amorphous SiO2-Al2O3
material shows a poor catalytic activity which correlates with the low accessibility of acid
centers. Among zeolites, mordenite leads to the highest epoxide conversion because of its high
aluminium content, but the activity per mol of active site is very low, probably because of
diffusional problems arising from the one-dimensional pore system of this zeolite. ZSM-5,
Al-TS-1 and Al-Ti-beta, which exhibit sites of intermediate acid strength, present a similar catalytic
activity, although Al-Ti-beta leads to a higher epoxide conversion due to its larger pore size.
Zn-containing zeolites, in particular CIT-6, catalyses selectively the formation of octen-1-ols. The
extension of the reaction over zeolitic materials seems to be influenced by limitations of both
pore and the crystal size of the catalysts. All mesoporous materials tested present much higher
activities per active site in comparison to those obtained with zeolitic materials, probably arising
from its larger pore sizes. The best catalytic activity has been obtained with Al-MCM-41
mesostructured materials presenting acid sites of medium acid strength.
Regarding to the product distribution, most of the catalysts tested promote the
isomerization of the epoxide towards the aldehyde and octen-1-ols through
carbocation-mediated processes. These octen-1-ols must be considered as interesting products as they can be
hydrogenated to terminal alcohols with a high added-value. Additionally, the absence of water
is a necessary requirement in order to avoid the nucleophilic attack of the oxirane ring with the
consequent formation of diol. Amorphous materials present poor selectivities to valuable
products with values close to 50%, whereas zeolites enhance the formation of the aldehyde
and/or octen-1-ols with selectivities to octanal+octen-1-ols higher than 60%. Al-TS-1 zeolite
other hand, Al-beta and CIT-6 lead mainly to octen-1-ols with values over 65%. The
homogeneous catalytic system leads to the formation of a high amount of aldehyde (59.8 %
selectivity), but with a low octen-1-ols selectivity. Al-MCM-41 synthesized by a sol-gel method
yield high selectivities to valuable products. In particular, sol-gel Al-MCM-41 catalyzes
selectively the isomerization of 1,2-epoxyoctante with selectivities to octaldehyde and
octen-1-ols of 40.6% and 44.7%, respectively. The high formation of octenocten-1-ols (in particular the allylic
alcohol) could result from the medium acid strength of these materials.
In summary, Al-MCM-41, prepared by the sol-gel method, is a material with
remarkable catalytic properties for the isomerization of long-straigth epoxides in liquid phase. It
presents a high surface area and, although its acidity is weaker than that of zeolites, the access
of the epoxide molecules to the active sites is not hindered as in the latter.
We gratefully acknowledge the financial support of this work by "Consejería de
Educación de la Comunidad de Madrid" (Contrato Programa Grupos Estratégicos de
1.M. Lenarda, L.Storaro, G. Renzo, J. Mol. Catal. 111 (1996) 203.
2.T. Onoda, Chemtech. September (1993) 34.
3.A. Johnstone, P.J. Middleton, W.R. Sanderson, WO Patent 95 100 243 (1995), to Solvay
4.S. Warwel, M. Klass, US Patent 5 321 158 (1994), to Solvay Interox GmbH.
5.K. Arata, K. Tanabe, Catal. Rev.-Sci. Eng. 25 (1983) 365.
6.I. Erden, Compr. Heterocycl. Chem. II (1996) 97.
7.J. Marc, Advanced Organic Chemistry, John Wiley Ed., New York, 1985.
8.W.F. Hölderich, J. Röseler, G. Heitmann, A.T. Liebens, Catal. Today 37 (1997) 353.
9.J.A. Elings, H.E.B. Lempers, R.A. Sheldon, Stud. Surf. Sci. Catal. 105 (1997) 1165.
R.A. Sheldon, H. van Bekkum (Ed.), Fine Chemicals through Heterogeneous Catalysis,
Wiley-VCH, Weinheim, 2001, p. 217.
R. Dimitrova, V. Minkov, N. Micheva, Appl. Catal. A 145 (1996) 49.
E. Ruiz-Hitzky, B. Casal, J. Catal. 92 (1985) 291.
M. Chamoumi, D. Brunel, P. Geneste, P. Moreaus, J. Solofo, Stud. Surf. Sci. Catal. 59
M. J. Faraj, US Patent 5 312 995 (1993), to Arco Chemical Technology.
W.F. Hölderich, N. Götz, L. Hupfer, H. Lermer, US Patent 4 980 511 (1987), to Basf AG.
D. Brunel, M. Chamoumi, P. Geneste, P. Moreau, J. Mol. Catal. 79 (1993) 297.
G.D. Yadav, D.V. Satoskar, J. Chem. Tech. Biotechnol. 69 (1997) 438
M.A. Uguina, G. Ovejero, R. van Grieken, D.P. Serrano, M. Camacho, J. Chem. Soc.,
Chem. Commun. (1994) 27.
G. Ovejero, R. van Grieken, M.A. Uguina, D.P. Serrano, J.A. Melero, Catal. Lett. 41
D.P. Serrano, M.A. Uguina, G. Ovejero, R. van Grieken, M. Camacho and J.A. Melero, J.
Mater. Chem. 9 (1999) 2899.
M.A. Camblor, A. Corma, S. Valencia, J. Mater. Chem. 8 (1998) 2137.
D.P. Serrano, R. van Grieken, M.E. Davis, J.A. Melero, A. Garcia, G. Morales, Chem Eur.
J. 8 (2002) 5153.
J. Aguado, D.P. Serrano, J.M. Escola, Microporous Mesoporous Mater. 34 (2000) 43.
W. Lin, Q. Cai, W. Pang, Y. Yue, B. Zon, Microporous Mesoporous Mater. 33 (1999) 217.
J. Aguado, D.P. Serrano, R. van Grieken, J.M. Escola, E. Garagorri, Stud. Surf. Sci. Catal.
135 (2001) 3915.
M. Kruk, M. Jaroniec, Chem. Mater. 12 (2000) 1961; R Ryoo, C.H. Ko, M. Kruk, V.
Antochshuk, M. Jaroniec, J. Phys. Chem. B. 104 (2000) 11465; C.G. Göltner, B. Smarsly,
B. Berton, M. Antonietti, Chem. Mater. 13 (2001) 1617; R. van Grieken, G. Calleja, G.D.
Stucky, J. A. Melero, R.A. Garcia, J. Iglesias, Langmuir 19 (2003) 3966.
G. Szöllösi, I. Kun, B. Török, M. Bartók, Stud. Surf. Sci. Catal. 125 (1999) 539.
W.F. Hölderich, N. Goetz, L. Hupfer, H. Lermer, US Patent 4 980 511 (1987), to Basf AG.
W.F. Hölderich, W.D. Mross, F. Merger, F. Fouquet, US Patent 4 929 765 (1984), to Basf